Polymer Colloid Science Jung-Hyun Kim Ph. D. Nanosphere Process & Technology Lab. Department of Chemical Engineering, Yonsei University National Research Laboratory Project the financialsupport of the Korea Institute of S&T Evaluation and Planning (KISTEP) made in the program year of 1999
What is a polymer colloids ? • Small polymer particles suspended in a continuous media (usually water) • EXAMPLES • - Latex paints • - Natural plant fluids such as natural • rubber latex • - Water-based adhesives • - Non-aqueous dispersions • COLLOIDS • - The world of forgotten dimensions • - Larger than molecules but too small to be seen in an optical microscope
What does the term “stability/coagulation imply? • There is no change in the number of particles with time. • A system is said to be colloidally unstable if collisions lead to the formation of aggregates; such a process is called coagulation or flocculation. • Two ways to prevent particles from forming aggregates with one another during their colliding • 1) Electrostatic stabilization by charged group on the particle surface • - Origin of the charged group • initiator fragment (COOH, OSO3-, NH4, OH, etc) • ionic surfactant (cationic or anionic) • ionic co-monomer (AA, MAA, etc) • 2) Steric stabilization by an adsorbed layer of some substance • 3) Solvation stabilization
Stabilization Mechanism • Electrostatic stabilization - Electrostatic stabilization Balancing the charge on the particle surface by the charges on small ions of opposite sign in the solution phase (counter ions) - Surface potential 1/x : Thickness of electrical double layer : dielectric constant of the medium I : Ionic strength • Steric stabilization - Hairy particles with uncharged hairs extending into nonaqueous medium as noncharged polymer chain • Electrosteric stabilization - Combination of electrostatic and steric stabilization by grafting to a polymer core particle polyelectrolyte chains
Forces Between Two Approaching Colloidal Particles • London-van der Waals force or dispersion force • Coulombic force associated with electrostatically charged particles • Force arising from solvation, adsorbed layers, etc.
Electrostatic Stabilization • Electrical double layer - Stern layer - Diffuse layer • Coulombic force - Electrostatic repulsion force to be dependent on the overlap of diffuse double layer - Potential energy of electrostatic repulsion, VR to be obtained by integration of repulsion force with respect to distance Figure. Schematic illustration of a negative charged spherical polymer latex particle with an electrical double layer. ---represents the range of influence of electrostatic forces. • London-van der Waals force - Potential energy of attraction, VA to be obtained by integration of attraction force with respect to distance
Electrostatic Stabilization • DLVO theory - Attraction decays as the inverse power of distance of separation. - Repulsion decays as an exponential of distance. - At both short and long distances of separation : Attraction > Repulsion - Critical coagulation concentration; a concentration at which the primary maximum becomes zero. • Advantages of electrostatic stabilization - Providing stability in nonaqueous systems where electrical effects are week. - Providing tolerance against high level of electrolyte - Stabilizing much greater particle concentrations • Disadvantages of electrostatic stabilization - Flocculation if coverage of particle is low
DLVO theory - Derjaguin and Landau(1941) and Verwey and Overbeek(1948) - Total potential energy of interaction - Potential energy of electrostatic repulsion - Potential energy of the van der Waals attraction
Steric Stabilization • Polymer must be strongly adsorbed at particle surface but not so strong as to be collapsed. • Polymer chains should extend as far as possible into solution - enhanced by solvent in which polymer is readily soluble. Figure. Schematic illustration of a noncharged polymer latex particle with adsorbed or grafted nonionic polymer chain. ---represents the range of influence of steric forces. • Most effective polymers are block copolymers; part strong acids and part weak acids.
Comparison of the Properties of Electrically and Sterically Stabilized Dispersion • Electrostatic Stabilization - Coagulates on addition of electrolyte - Mainly effective in aqueous dispersion media - Coagulation often irreversible - Freezing often induces irreversible coagulation • Steric Stabilization - Insensitive to electrolyte - Equally effective in aqueous and non-aqueous dispersion media - Equally effective at high and low volume concentration - Reversible flocculation common - Good freeze-thaw stability
Table. The differential types of heterogeneous polymerization systems
Dispersion polymerization • Constitution • - Initiator : water or oil soluble • - Continuous phase : water, alcohol, solvents • - Discrete phase : initially absent, monomer • -swollen polymer particles form • - Steric stabilizer • Characteristics • - In the medium : monomer & initiator is • soluble, polymer is precipitated • - Initiation : in the medium and inside the particles • - Occurrence of phase separation at an early stage : • the formation of primary particles • - Particles are swollen by a mixture of the monomer and the medium • - Typical particle radius : more than 1 ㎛
Suspension polymerization • O/W suspension polymerization monomer (oil-soluble) Discrete phase initiator (soluble in the monomer) chain transfer agent(oil-soluble) Suspension medium water - Initiator & monomer : insoluble in the suspension medium - The volume ratio of the monomer to water : 0.1-0.5 - Typical particle radius : > 1 ㎛ - Polymer particles obtained by suspension polymerization have a relatively broader size distribution • W/O suspension polymerization - Inverse suspension polymerization - The suspension medium : a water immiscible liquid (toluene, dichloroethane, etc) - Monomer & initiator : soluble in water - Diluent : water or highly polar organic liquid
O/W suspension polymerization - Constitution Water : medium Initiator : soluble in the monomer, insoluble in the medium Monomer : insoluble in the medium Stabilizer - Controlling variables of particle size Reactor and process type Stirring rate Monomer/water ratio Nature and concentration of stabilizer Rate of polymerization - Diluted O/W suspension polymerization Monomer is diluted with a water-immiscible liquid (diluent) Suspension polymerization
Suspension polymerization • Suspension process of poly(vinyl chloride) • Components • vinyl chloride 3500 (g) • water 5000 (g) • surfactant/stabilizer 0.7 (g) • poly(vinyl alcohol) 3.5 (g) • lauroyl peroxide 1.5 (g) Fig. Schematic diagram of suspension polymerization of poly(vinyl chloride)
Emulsion polymerization • Production • Billions of metric tons/year • Advantage • - High rate of polymerization • - High molecular weights • - Low viscosity • - Excellent heat transfer • - High conversions • - Continuous production possibility
Emulsion polymerization • Characteristics of emulsion polymerization A. Water-immiscible monomer emulsified in water using oil-in-water emulsifier and polymerized using a water-soluble or oil-soluble initiator B. Product is a colloidal dispersion of submicroscopic polymer particles in water : Average diameter usually 0.1-0.3 ㎛ C. Monomer emulsion droplet size : usually 1-10 ㎛ D. Proposed mechanism for initiation of polymerization 1. Monomer-swollen micelles 2. Adsorbed emulsifier layer 3. Aqueous phase 4. Monomer droplets
initiator aqueous-phase propagation aqueous-phase termination entry R• propagation termination transfer propagation oligomer M• aqueous-phase termination exit M• re-entry re-escape M• propagation termination Emulsion polymerization Fig. The various events that occur subsequent to initiator dissociation in an emulsion polymerization. Note particularly the aqueous- phase event : propagation and termination, both of radicals derived directly from initiator from initiator and of those arising from exit
Important considerations in emulsion polymerization 4. Particle morphology A. Uniform B. Core-shell C. Aggregate of smaller particles 5. Molecular properties A. Molecular composition B. Molecular weights C. Molecular architecture 6. Transport and distribution of recipe ingredients A. Free radicals B. Emulsifier C. Monomer 1. Particle formations A. Emulsifier micelles B. Homogeneous nucleation C. Monomer droplets D. Flocculation of primary particles 2. Particle growth A. Internal polymerization a. Small volume reactor b. Gel-effect at high conversion B. Flocculation a. Deposition of smaller particles b. Flocculation among mature particles C. Shrinkage of particles at high conversions 3. Particle stabilization A. Added emulsifier B. Effects of initiator end groups C. Functional monomers
Comparison between Conventional Emulsion Polymerization and Inverse Emulsion Polymerization Conventional Emulsion Polymerization • Water-immiscible monomer emulsified in water using oil-in-water emulsifier • and polymerized using a water-soluble or oil-in-soluble initiator. • Product is a colloidal dispersion of submicroscopic polymer particles in water • : Average diameter usually 0.1~0.3 m • Monomer emulsion droplet size usually 1~10 m. • Proposed mechanism for initiation of polymerization • 1. Monomer-swollen micelles • 2. Adsorbed emulsifier layer • 3. Aqueous phase • 4. Monomer droplets Inverse Emulsion Polymerization • Water-soluble monomer, usually in aqueous solution, emulsified in continuous • oil phase using water-in-oil emulsifier and polymerized using an oil-soluble or • water-soluble initiator. • A Product is a colloidal dispersion of submicroscopic polymer particles, often • swollen with water-in-oil : Average diameter usually 0.05~0.31 m
Miniemulsion polymerization • Monomer droplet : • - 100-500 nm • - Similar to latex particle size • - Significant loci for nucleation • and polymerization • Additive (fatty alcohol or alkane) : • - To stabilize emulsion • - To decrease the droplet size • - To increase amount of adsorbed • emulsifier • - No relationship with kinetics
Application Fields of Colloids Area Example Paints, Adhesives, Floor polishes, Print inks, Carpet backing, Paper sizing, Water/sewage treatment, Secondary oil recovery, Rubberized concrete Size standard for electron microscopy High resolution chromatography column packing Magnetic particles targeted drug delivery Immunodiagnostics Controlled released drugs Catalysts, Colloids & surface chemistry, Coagulation kinetics Model liquid crystals, Rheology, Dielectric spectroscopy Particle interaction *Dispersion forces *Electrostatics *Steric stabilization Industrial Research Medical Chemical
PROGRESS & KINETICS OF EMULSION POLYMERIZATION
Three stage of emulsion polymerization • Interval I : Particle initiation stage • - Continuous until micelles have disappeared • Interval II : Particle growth stage • - Constant number of particles plus monomer emulsion droplets • - Particles grow until monomer droplet phase disappears and • all monomer is in the particles • Interval III : Particle growth stage • - Particles grow until monomer is completely polymerized • or initiator is exhausted
INTERVAL 1 Monomer droplet Free radical Surfactant Initiator Iatex particle micelle INTERVAL 2 Monomer droplet INTERVAL 3 Fig. The three Intervals of emulsion polymerization
Kinetics of emulsion polymerization • Polymerization rate • Steady state (initiation rate = termination rate) • Rp = kp[R • ] [M] [R • ] : unknown radical concentration • - Assumption : Rate of formation and destruction is equal • Ri = ki [I2]= Rt = kt [R • ]2 • Kinetic chain length v : 활성 사슬당 소요된 단량체의 수로 정의 • v = Rp / Ri = Rp / Ri
Kinetics of emulsion polymerization • Polymerization rate • Disproportion termination Xn = υ • Combination termination Xn = 2υ • Case in transfer reaction Xn : (rate of proportion) / (sum of the rates of all reactions leading to polymer molecules) • Rate of emulsion polymerization
The rate of polymerization : the product of the conc. Of active particles : the product of the conc. Of active particles : the average # of radicals per micelle plus particle This eq. Applies to Interval II and III where only polymer particles exist (no micelles) The value of during Interval II and III is of critical importance in determining Rp.
Degree of Polymerization The rate ri at which primary radicals enter a polymer particle The same as the rate of termination rt of a polymer chain for Case 2 behavior The degree of polymerization is the rate of growth of a polymer chain divided by the rate at which primary radicals enter the polymer particle. The degree of polymerization in an emulsion polymerization is synonymous with the kinetic chain length. The rate and degree of polymerization can be simultaneously increased by increasing the number of polymer particles at a constant initiation rate.
Number of Polymer Particles The number of polymer particles is the prime determinant of the rate and degree of polymerization since it appears as the first power in both Eq 4-5 and 4-7 The number of particles that can be stabilized is dependent on the total surface area of surfactant present in the system The practical viewpoint one can simultaneously increase and by increasing N. The predicted dependence ofN and S and Ri for the formation of polymer particles by micellar and homogeneous nucleation followed by coagulative nucleation is given as follows
Nucleation Mechanism • Micellar Nucleation Fig. Emulsion polymerization during interval (2), the number of micelles, particles, and droplets are arbitrary; d is diameter
Micellar Nucleation • Example of micellar nucleation scheme
Homogeneous Nucleation Mechanism Fig. Schematic of the homogeneous nucleation theory
Homogeneous Nucleation Mechanism • Appreciable water soluble monomer • Free radicals generated in aqueous phase • Formation of 'primary' particles • Propagation • Flocculation • Emulsifier-free emulsion polymerization • Stability : Electrostatic stabilization of initiator portion
Coagulative Nucleation Mechanism • Two step nucleation (Napper & Gilbert) - First step ; 'precursor' particle formulation - Second step ; 'mature' particle formulation by aggregation of precursor particle
SO4-• + M propagation coagulation propagation M M M jcrit precipitation entry termination precursor particle Mature particle Z propagation • Coagulative Nucleation Mechanism Fig. More detailed illustration of the homogeneous coagulative (HUFT) nucleation description of particle formation, which dominates for surfactant concentrations below the cmc.
Nucleation in Monomer Droplet • Monomer droplet : • 1 - 10 ㎛ size • Small number Small surface area • Capture size • Decrease size of monomer droplet 100 - 500 nm size • Miniemulsion & Microemulsion polymerization • Final latex particle size ; • Initial droplet size
Nucleation in Monomer Droplet • Role of additives in miniemulsion - Formation & stabilization of small size droplet • adsorption of emulsifier • - Increase of monomer-swollen ratio • - Decrease equilibrium concentration of monomer in monomer droplet • Microemulsion polymerization • - Initial droplet size : 5 - 40 nm • - Increase of polymerization rate • - Interval I : Until microemulsion droplet disappeared • - Interval II : Until polymerization rate decreases • - High M.W. polymer formation
Other Considerations of Emulsion Polymerization
Variation common to most polymerization process : • - Monomer mixture • - Programmed addition • - Other ingredients : solvent, CTA, dissolved polymer etc. • - Molecular weight characteristics • - Grafting • Additional variations possible with emulsion polymerization : • - Particle size characteristics • - Particle morphology • - Composition variations • within individual particles • among particles of different size • - Particle surface characteristics • - Rheology : particle contributions, continuous phase contributions • interfacial phenomena • - Continuous phase characteristics
Development sequence for polymer latex systems Selection of Monomer System Tg, MFFT, Durability, Water Properties Choice of surfactant Type, Level, CMC, HLB Catalyst System and Polymerization Temperature Control, Molecular Weight Conditions